- Nano Express
- Open Access
Nanoscale Au-ZnO Heterostructure Developed by Atomic Layer Deposition Towards Amperometric H2O2 Detection
Nanoscale Research Letters volume 15, Article number: 41 (2020)
Nanoscale Au-ZnO heterostructures were fabricated on 4-in. SiO2/Si wafers by the atomic layer deposition (ALD) technique. Developed Au-ZnO heterostructures after post-deposition annealing at 250 °C were tested for amperometric hydrogen peroxide (H2O2) detection. The surface morphology and nanostructure of Au-ZnO heterostructures were examined by field emission scanning electron microscopy (FE-SEM), Raman spectroscopy, atomic force microscopy (AFM), X-ray photoelectron spectroscopy (XPS), etc. Additionally, the electrochemical behavior of Au-ZnO heterostructures towards H2O2 sensing under various conditions is assessed by chronoamperometry and electrochemical impedance spectroscopy (EIS). The results showed that ALD-fabricated Au-ZnO heterostructures exhibited one of the highest sensitivities of 0.53 μA μM−1 cm−2, the widest linear H2O2 detection range of 1.0 μM–120 mM, a low limit of detection (LOD) of 0.78 μM, excellent selectivity under the normal operation conditions, and great long-term stability. Utilization of the ALD deposition method opens up a unique opportunity for the improvement of the various capabilities of the devices based on Au-ZnO heterostructures for amperometric detection of different chemicals.
The development of different nanoscale two-dimensional (2D) heterostructures for their usage in various electrochemical devices is modern and established trend during the last decade of the twenty-first century [1,2,3,4,5]. So far, several technologies have been dominated in this trend including RF sputtering, chemical vapor deposition (CVD), hydrothermal method, solvothermal method, thermal evaporation, sol-gel, mechanical exfoliation, etc. [5, 6]. However, it was clearly stated in the recent review  that the ALD as an emerging technology has not yet fully exploited its features towards the development of reliable electrodes for the measuring devices. There are several reasons for that including the availability of precursors, specific ALD temperature window for deposition, lack of reliable recipes, etc. However, on the other hand, the advantages of ALD are far superior to the existing capabilities of other techniques . First of all, ALD is the only one technology, which enables fabrication of conformal, defect-free semiconductor 2D nano-films and their heterostructures on the wafer scale with precise control of their thickness during fabrication at the Ångstrom level . In this regard, state-of-the-art nanoscale interfacing and molecular engineering of the sensing electrode materials can open up completely new possibilities by providing ultra-thin channels for key doping, minimization of the density of interfacial impurities and optimization of sensing capabilities of the devices . Several recent reports about ALD-developed wafer-scaled monolayers of WO3 [8, 10, 11] and TiO2 [12, 13] and few-layered MoO3 [14, 15], TiO2 , and their heterojunctions including Au-WO3-TiO2 , Ga2O3-WO3 , Au-Ga2O3-TiO2 , etc. are recent consecutive evidence of the impact of this technology on the extension of capabilities of materials for electrochemical , optical , and photovoltaic devices .
H2O2 possesses strong oxidizing and reducing properties and has been extensively used in various applications including different chemical, pharmaceutical and mining, textile, and clinic industries . H2O2 is also a by-product of enzymatic reactions and its accurate and sensitive detection has been required in food, environmental, and pharmaceutical applications. Consequently, it is critical to detect H2O2 rapidly and selectively particular at the low concentrations level. So far several methods have already been established for fast H2O2 detection including colorimetric [22,23,24,25], non-enzymatic [26, 27], electrochemical [28,29,30,31,32,33,34,35], chemiluminescent [36,37,38,39], and fluorometric [39, 40] measurements. Although all of them demonstrated reasonable results and good repeatability, their main disadvantages include complex separation processes, time-consuming derivation and relatively high running cost. In addition, due to the electro-active nature of H2O2, non-enzymatic electrochemical detection method can be considered as a valuable alternative for selective H2O2 detection  considering that it possesses the rapid response with great stability, wide linear detection range, high precision, low cost, and simplicity . In fact, owing to the extremely high surface-to-volume ratio in 2D nanomaterials and heterostructures, their employment for such non-enzymatic H2O2 detection is highly desirable . It was proven that the heterostructured and sandwiched nanomaterials have better analytical sensing performance than the ordinary nanomaterials . On the other hand, their surface functionalization enabled them to increase substantially their sensing capabilities  ensuring the development of a combination of two or more dissimilar nano-materials to form the hybrid nanocomposites, especially metal-semiconductor hybrids . Thus, the outstanding properties of Au-ZnO heterostructures for enhancing the analytical sensing performance of electrochemical sensors are due to the following: (i) the Schottky contacted between nanostructured Au and ZnO results in generation of the thicker depletion layer at the Au/ZnO interface compared with the bare ZnO nanostructure; (ii) the inert surface nature of ZnO; and (iii) high selectivity of Au co-catalyst for direct 2e− reaction, which maximizes the H2O2 detection. For instance, Au-semiconductor hetero-interfaces have a critical effect on the properties of the surface layer particularly if the thickness of such a layer is just a few nanometers. In this regard, ALD technology is imperative for fabrication of the wafer-scaled semiconductors with nanometer thickness. Moreover, ZnO with wurtzite hexagonal structure has been considered as a very promising candidate for the development of such hetero-interfaces. It has a very wide (~ 3.37 eV) bandgap and can be fabricated defect free by ALD . So far, nanoscale ZnO has clearly demonstrated unique properties as well as excellent electrochemical capabilities in photovoltaics, catalysts, batteries, and different chemical sensors [47,48,49,50,51,52,53]. However, despite outstanding reported properties and wide usage of ZnO in many applications, Au-ZnO heterostructures have not yet been reported for electrochemical H2O2 sensing.
In this work, wafer-scale 2D Au-ZnO heterostructures were developed by the ALD technique using (C2H5)2Zn and H2O precursors, as presented in Fig. 1, and the best deposition parameters were established and summarized in Table 1. Both physical and electrochemical properties of fabricated Au-ZnO heterostructures towards amperometric H2O2 detection at the low and high H2O2 concentration levels were subsequently investigated. It was confirmed that the ALD-developed Au-ZnO heterostructures demonstrated high sensitivity and selectivity as well as great long-term stability for the wide linear range of H2O2 concentrations (1.0 μM to 120 mM), which ensured a great potential for their further implementation in practical electrochemical devices.
2D Au-ZnO Heterostructures
Four-inch Si/SiO2 wafers (12 Ω/cm) were used as substrates for ALD depositions of ZnO. It should be mentioned that in order to reduce the potential influence of Si wafer on the subsequent electrical measurements, insulating SiO2 layer with a thickness of approximately ~ 100 nm was CVD on all wafers. The CVD of SiO2 was done prior to ZnO ALD deposition employing Oxford Instruments PLASMALAB 100. After that, gold (Au) electrodes were fabricated on the developed thick SiO2 surface by using optical photo-masks and electron beam evaporation (EBE) (Nanochrome II (Intivac)). Au electrodes were grouped into square 3-electrode structures, which was made on the SiO2/Si wafer segments as shown in Fig. 1a. The thickness of all Au electrodes was about ~ 150 nm, which was confirmed by appropriate AFM measurements (See Additional file 1: Figure S1 of Supporting Information). Then, thin-film ZnO were deposited on the top of these Au electrodes by ALD. All wafer-scale ZnO depositions were performed on Savannah S100 (Ultratech/Cambridge Nanotech) equipment. The chamber was heated up to 250 °C. The main precursor—solid diethylzinc [(C2H5)2Zn] (99%, Strem Chemicals)—was heated to 250 °C. Then, H2O vapor was used as a second precursor. The thickness of both the CVD SiO2 and the growing ZnO films was in situ monitored by spectroscopic ellipsometry (SE) (J.A. Woollam M-2000) over the wavelengths of 250–1690 nm. Specifically, Fig. 1a depicts the angular image of 2D ZnO on the specially designed Au electrodes EBE on 4-in. SiO2/Si wafer straight after ZnO deposition. Developed 2D ZnO films appeared to be fully transparent. Subsequent to the ZnO deposition, all SiO2/Si wafers were diced into the small segments presented as an insert in Fig. 1a for further post-annealing. Both experimental and model-generated data for variable angle SE measurements of CVD deposited SiO2 on Si wafer with SE mapping of the thickness of SiO2 in Ångstrom are shown in Fig. 1b. The Cauchy model is used for fitting the SE data in order to obtain the optical properties.
Graphical interpretation of both [(C2H5)2Zn] and H2O precursors and experimental data for SE SiO2 thickness mapping in Ångstrom are depicted in Fig. 1c and d, respectively. Additional experimental and model-generated data for variable angle SE measurements of ZnO films with an initial thickness of 0.9 and 1.3 nm, respectively, are summarized in Additional file 1: Figure S2 of Supporting Information. In order to ensure the consistency of ALD fabricating ZnO films, several trials carried out at the deposition temperature of 250 °C. Uniformly distributed, defects-free, conformal wafer-scaled ZnO films were obtained. For example, Fig. 1e shows the SE measurements for ~ 1.3-nm-thick ZnO film prior to annealing. As clearly presented in this figure the thickness of approximately 1.3 nm of ZnO film was impeccably distributed over 4-in. SiO2/Si wafer. Thus, these ZnO films were selected for post-annealing and further electrochemical H2O2 detection. In such ultra-thin ZnO nanostructures the (10-10), (11-20), and (0001) planes are repeating the unit cell in the appropriate directions. In this case, wurtzite crystal structure of ZnO from orthorhombic unit cell is obtained , as schematically presented in Fig. 1 f. Although all of the planes have non-uniform atomic arrangements, the zigzag pattern of the Zn and O sub-lattices overlaps for the (10-10) and (11-20) planes, whereas the sub-lattices along the c-direction for the (0001) plane are slightly shifted . Such shift divides the weight center of negative and positive charges, and consequently, enables polarity of the layers. The developed recipe, including the established deposition parameters for ALD fabrication of ZnO films, is summarized in Table 1.
Finally, after ZnO deposition on Au electrodes, the Au-ZnO heterojunctions were made on each segment of the wafer (insert in Fig. 1a) in the heating chamber. For this purpose, all fabricated ZnO films with a thickness of ~ 1.3 nm deposited Au electrodes were heated up to the temperature of 250 °C in air for the development of Au-ZnO heterostructures. The heating rate was 0.5 °C/min. At such annealing temperature and at the absence of any molecular charge compensation mechanism, the polar surfaces of ZnO are unstable and thus undergo surface reconstructions and agglomeration into island-like nanostructures significantly enhancing the surface-to-volume ratio of Au-ZnO heterostructures. Then, after annealing, the developed Au-ZnO heterostructures were utilized for further materials characterization experiments. Thus, unless it is stated otherwise, these heterostructures were subsequently used for amperometric H2O2 detection.
The surface morphology of Au-ZnO heterostructures was investigated by FE-SEM (JEOL 7800F) and by AFM (JPK System, Nano Wizard). XPS measurements were used for establishment the chemical state and surface composition of the developed heterostructures (Rigakudenki model, 7000 with monochromatic Mg-Kα radiation at 300 W). Binding energy of 284.6 eV for C 1 s is utilized for calibration and correction of the obtained binding energy values. In addition, Raman spectroscopy measurements were used to determine the vibrational modes of molecules, identify the crystallinity of developed heterostructures and their structural fingerprint. They were performed on (Lab Ram ARAMIS, Horiba Jobin-Yvon, Edison) Raman spectrometer equipped with λ = 532.2 nm Ar-ion laser. The lattice vibrations of ZnO were investigated and recorded by Fourier transform infrared spectroscopy (FTIR) spectrometer (Shimadzu IR Prestige 21). H2O2 sensing properties of the developed Au-ZnO heterostructures were electrochemically measured at the room temperature on Autolab PGSTAT204 (Metrohm Autolab, B.V.). For this purpose 3-electrode system is designed. In this system, Pt wire represents the counter electrode, Au-ZnO heterostructure with the area of 0.5 cm2 acts as the working electrode, and Ag/AgCl (3.0 M KCl) used as the reference electrode, respectively. The potential range from − 0.9 to 0.2 V was used for current-voltage (CV) measurements at the room temperature of 20 °C. In addition, both chronoamperometry and EIS measurements were used at various conditions for electrochemical behavior evaluation of ALD-fabricated Au-ZnO heterostructures. Specifically, an applied potential of 0.14 V was utilized for chronoamperometry, where the H2O2 concentration was gradually increased stepwise at the magnetic stirring of 330 rpm. Moreover, EIS experiments were performed in 1 mM K4Fe(CN)6 solution containing 0.1 M KCl. In these experiments, the frequency changed from 0.1 to 105 Hz.
Results and discussion
Characteristics of Au-ZnO heterostructures
Figure 2 combines both AFM and FE-SEM images representing the established morphology of Au electrodes and developed Au-ZnO heterostructures, respectively, after post-deposition annealing at 250 °C for 3 h. Specifically, Fig. 2a shows the AFM measurement of the flat Au electrode on Si/SiO2 wafer prior to annealing. It was evidently observed in this electrode that the average size of Au nanoparticles was about ~ 50–80 nm and their average height was approximately 3.0 nm. The uniform and smooth distribution of all Au nanoparticles on the surface of the SiO2/Si substrate was observed. On the contrary, Fig. 2b shows FE-SEM picture of the surface morphology of Au-ZnO heterostructures after post-annealing at 250 °C. Compared with the similar thickness of annealed ultra-thin WO3  and TiO2  films deposited by ALD, the FE-SEM image of Au-ZnO heterostructures depicts quite a rough surface. It is clearly visible that the ZnO films due to their extremely thin thickness were broken, aggregated, and finally agglomerated into island-like Au-ZnO heterostructures under the high annealing temperature. Nevertheless, similar results for ALD-fabricated monolayer WO3 were reported . The reason for the development of such an island-like structure is the selection of the deposition temperature within the ALD window for (C2H5)2Zn precursor and the annealing time. The deposition temperature of 250 °C for (C2H5)2Zn precursor testifies for the bigger ZnO grain deposition and was consistent with the previous report . Furthermore, the post-annealing alters stoichiometry, charge carriers concentration, and their mobility. It is also enhanced the surface-to-volume ratio of the developed heterostructures ensuring their high electrochemical sensitivity towards the measuring chemical . Thus, the overall properties of the nanometer-thick ZnO films deposited on Au electrodes are determined not only by the parameters of the ALD process but also by the post-growth treatment such as thermal annealing. Moreover, the impact of annealing time of post-annealing of ZnO films on their developed properties was properly evaluated . Noteworthy, the size of obtained ZnO nano-grains in the Au-ZnO heterostructures in our investigation was consistent with the published results for the chosen annealing time . Meanwhile, Fig. 2c represents the lattice vibrations in the perturbation area of FTIR measurements for both pure ZnO powder and ALD-fabricated ZnO film with a thickness of 1.3 nm. Peaks of 464 and 472 cm−1, representing the Zn-O stretching vibrations for the tetrahedral surrounding of Zn atoms , were collected for the 1.3-nm-thick ZnO film and commercial ZnO powder, respectively. As is demonstrated in Fig. 2c, the peak for the ALD-fabricated 1.3-nm-thick ZnO film was slightly shifted compared with the same peak measured for the commercial ZnO powder and was consistent with previous analysis . Considering the possibility that the nanostructured ZnO may not be stable in either acidic or base solutions, additional FE-SEM measurements of Au-ZnO heterostructures after their long-term stability tests (more than 30 consecutive days of testing) were also taken place. The obtained FE-SEM images for Au-ZnO heterostructures (Fig. 2d) have clearly confirmed and testified that the surface morphology of samples used for the long-term stability tests has not been changed.
Unfortunately, the employment of a well-established X-ray diffraction technique for crystallinity characterization of the developed Au-ZnO heterostructures was not possible owing to their extremely thin thickness. Therefore, the surface-sensitive quantitative spectroscopic XPS measurements were performed on such heterostructures to establish the elemental composition at the parts per thousand range and chemical and electronic states of the elements that exist within the heterostructure. A wide-scan survey spectrum of the developed Au-ZnO heterostructures is displayed in Fig. 3a, where the main Au, O, and Zn elements can be clearly identified. A survey spectrum is usually the starting point of XPS analyses because it shows all elements present on the sample surface. The spectrum was calibrated using the C 1 s peak at 284.8 eV. Peaks of Au 4d, Au 4f, and C 1 s are also present in the survey, which reflected from the Au electrode and calibration reference for binding energies of the peaks, respectively. The high-resolution scan of Zn 2p is presented in Fig. 3b. The doublets of Zn 2p3/2 and Zn 2p1/2 were displayed at 1021.6 and 1044.8 eV, respectively. The binding energy difference of 23.2 eV between these two Zn 2p3/2 and Zn 2p1/2 peaks confirmed the presence of zinc in Zn2+ state [57, 58] within the heterostructure. Moreover, the results obtained are very consistent with the previously reported parameters for ZnO thin films . The high-resolution scan for Au 4f and Zn 3P is depicted in Fig. 3c. Two deconvoluted peaks of Au 4f7/2 and Au 4f5/2 have a close similarity to the respective binding energies at 83.5 and 87.2 eV in the Au 4f core-level spectrum for the developed Au-ZnO heterostructure. Characteristically, the ~ 3.7-eV separation between the maximum intensity of the peaks at 83.5 and 87.2 eV perceived in the Au-ZnO heterostructure could be ascribed to the spin-orbit components Au 4f7/2 and Au 4f5/2 of the metallic gold [59,60,61,62,63]. Quite intriguing was the fact that the recorded 3.7-eV peak separation is very similar to the separation of the same peaks in the previous report . Both Au 4f7/2 Au 4f5/2 peaks exhibited the downward shift in binding energy accompanied by the increase in Au incorporation for Au° and Au+ states. In addition, two very weak peaks corresponding to Zn 3p3/2 and Zn 3p1/2 were also readable at 88.6 and 91.3 eV, respectively.
The O 1 s spectrum of Au-ZnO heterostructures is shown in Fig. 3d. Typically, for O 1 s peaks in heterostructures, the obtained O 1 s peaks for Au-ZnO heterostructure are deconvoluted into 3 major sub-peaks. For instance, the peak at 530.2 eV is assigned to O2− ions of Zn-O bonding reported for the wurtzite ZnO structure . Another peak at 532.1 eV is ascribed to both O− and O2− ions in the oxygen-deficient regions of the ZnO matrix. Remarkably, the intensity of these peaks partially associated with the changes in the oxygen vacancy concentration . In addition, peak at 530.0 eV is a reflection of the adsorption of O2, H2O, and CO2 oxygen-containing molecules on the Au-ZnO heterostructure surface . It should be stressed that the binding energies of the observed 3 sub-peaks are coherent with the previously published Gaussian peaks at ~ 530.2, 531.1, and 532 eV, respectively .
Raman spectroscopy is a contactless and non-destructive material quality analyzing technique. It was employed for the analysis of the phase orientation, transport, and vibration properties. Thus, the recorded Raman spectrum for ALD-fabricated ZnO film with a thickness of 1.3 nm is presented in Fig. 4a. Equally important, the Raman spectrum for the commercial ZnO powder is also incorporated into Fig. 4a for comparison. The main characteristic helping to identify the wurtzite ZnO phase is a non-polar phonon mode (E2high) connected to the lattice vibration of the O2 atoms observed at ~ 430 cm−1. It is interrelated to the lattice vibrations of Zn atoms . Other E2high phonon modes for the ZnO powder were noticed at ~ 438.9 and 440.4 cm−1, respectively. It is quite prominent that the observed E2high phonon mode depicted in Fig. 4a shifted from its standard value (437 cm−1), appeared to designate the existence of compressive strain in ZnO powder as well as in ALD fabricated 2D ZnO film. However, compared with the ZnO powder, 3 additional peaks at ~ 259, 570, and 684 cm−1 for 2D ZnO film were recorded. Specifically, a high intensity of the peak at 570 cm−1 is noticeable, which can be attributed to the high concentration of the developed oxygen vacancies in ZnO nanostructure . Noteworthy, this mode is absent in the spectrum for ZnO powder. However, in our case, the observed intensity of the 570-cm−1 peak is too high, which may also be ascribed to the overlapping A1(LO) and E1(LO) phonon modes. Considering the fact that the surface optical modes are usually observed between the A1(TO) and A1(LO) polar phonon modes , the huge intensity of the peak at 570 cm−1 could also be assigned to the intrinsic defects of the host-lattice induced by the development of the heterostructure [68,69,70]. Nevertheless, our investigation confirmed that the ALD fabricated 2D ZnO films possess high crystalline and optical properties in contrast to the commercial ZnO powder. Furthermore, the influence of the point defects which appeared in the 2D ZnO films on the anomalous intensity of the Raman modes can be disregarded.
Figure 4b expresses plotted impedance spectra of both wafer substrate and Au-ZnO heterostructure. The impedance results for the substrate as well as for the Au-ZnO heterostructure were obtained using the Randles equivalent circuit. The temperature of the buffer 5 mM K4Fe(CN)6 solution was 25 °C. The large Nyquist plot with Ret = ~ 1.5 kΩ was recorded for the Au-ZnO heterostructure, while the smaller Nyquist semicircle with Ret = ~ 0.9 kΩ was measured for the wafer substrate. Although the thickness of the Au-ZnO heterostructure was very thin, its contribution to the overall heterostructural impedance was found to be substantial and noticeable.
H2O2 sensing properties
The electrochemical performance of the sensor based on Au-ZnO heterostructures with an area of approximately 1.0 cm2 towards H2O2 was performed using the 3-electrode system, as presented in detail in the “Methods” section. Remarkable improvement towards amperometric H2O2 detection was clearly observed between the blank substrate and the sensor based on Au-ZnO heterostructure, as shown in Fig. 5a. In order to investigate it further, CV measurements at the different H2O2 concentrations (Fig. 5b) continued until the upper detection limit of 120 mM was established. Figure 5c displays great linearity between the recorded peak current and the measured H2O2 concentration, which reaffirmed the effective electro-catalytic activity of Au-ZnO heterostructures. A fast response-recovery time of approximately ~ 2.0 s for the amperometric H2O2 detection was obtained. This response-recovery time indirectly resonated rapid electron transfer reactions at the Au-ZnO heterostructures. It could be also due to the high concentration of the oxygen vacancies on the heterostructure surface. Noteworthy, the EIS measurements, presented in Fig. 5d, showed that as the H2O2 concentration in the K4Fe(CN)6 solution increased, the measured Nyquist plot is gradually getting to be smaller and the Ret value proportionally decreased, which indicates the improved electron transfer rate. It should be stressed that the low Ret is an indirect confirmation of the presence of diffusion-limited process between the Au-ZnO heterostructure surface and the 5 mM K4Fe(CN)6 solution . The correlated linear regression equation could be presented as follows: EP (V) = 0.0671 logν + 0.278. For the diffusion-controlled process mentioned above, EP can be defined by the following Tafel equation :
where R is the universal gas constant , T is the temperature of the solution measured in K, F is the Faraday constant, α is the electron transfer coefficient, nα is the number of electron transfers involved in the rate-determining step, and K is a constant.
Moreover, chronoamperometry as a time-dependent technique is utilized for the determination of the following parameters of amperometric sensors based on Au-ZnO heterostructures: sensitivity, linear response range and the low limit of detection (LOD) for H2O2. In this technique, a square-wave potential is applied to the working electrode. The electrode current, measured as a function of time, fluctuates according to the diffusion of H2O2 from the bulk solution towards the Au-ZnO heterostructure surface. As the current is integrated over the relatively longer time intervals, chronoamperometry provides a better signal-to-noise ratio compared with other amperometric techniques. Therefore, chronoamperometric measurements were performed for Au-ZnO heterostructures and the main results are summarized and presented in Fig. 5e. During these measurements, the H2O2 was added approximately every 50 s. It is clear from Fig. 5e that the sensor based on Au-ZnO heterostructures demonstrated typical current time dynamic responses at changes of concentration from 2.0 μm to 106.5 mM. Responses to much lower H2O2 concentrations from ~ 1.0 to 1100 μM are shown as insert to Fig. 5e. The response time to the various H2O2 concentrations was found from i–t curves. In fact, the Au-ZnO heterostructures have clearly demonstrated the fastest response-recovery time (~ 2.0 s) among all reported ZnO-based electrochemical H2O2 sensors [28,29,30,31,32,33,34,35]. Corresponding calibration curve for H2O2 detection by 2D Au-ZnO heterostructures is presented in Fig. 5 f. Noteworthy, the sensor based on Au-ZnO heterostructures signified the remarkable linear dependence of chronoamperometric responses within the wide H2O2 concentrations range of ~ 1.0 μm–120 mM. It must be stressed that such a wide linear range for the sensor based on ALD-fabricated Au-ZnO heterostructure is the widest linear range among all electrochemical [28,29,30,31,32,33,34,35], chemiluminescent [36, 37, 72], colorimetric [23,24,25], and fluorometric [37,38,39,40] H2O2 detectors reported to date. In addition to the widest linear measured H2O2 concentrations range and extremely fast response-recovery time, the low LOD of 0.78 mM was achieved for the Au-ZnO heterostructures. This low LOD value is compatible with the best LOD values reported for colorimetric [23,24,25] and fluorometric  H2O2 sensors and is better than the reported LOD value for chemiluminescent [36, 37] H2O2 detectors. Therefore, the experimental results obtained for Au-ZnO heterostructures have unambitiously verified that these ALD-fabricated heterostructures possess excellent sensing capabilities towards amperometric measurements of the lower H2O2 concentrations compared not only to the ZnO-based nanostructures but also to the best other H2O2 detection methods. All characteristics for 2D nano-films and heterostructures reported so far for electrochemical, chemiluminescent, colorimetric, and fluorometric H2O2 detectors are summarized into Table 2.
Besides the widest linear H2O2 concentration range, low LOD, and the fast response-recovery time, the cross-reference of Au-ZnO heterostructures to the other chemical agents existing in the measuring solution has also been evaluated at room temperature. For this purpose, 1.0 mM of the different chemicals were subsequently introduced into the measuring solution containing 10 μM H2O2. Responses of 2D Au-ZnO-heterostructures to the different interfering agents including glucose, KCl, NaNO2, AA, UA, and KNO3 are displayed in Fig. 6a. It should be stressed that the concentration of the additional chemicals was about 100 times higher (1000 μM) and about 50 times higher for glucose (500 μM) than the existing H2O2 concentration (10 μM) in the solution. Each interfering chemical agent was tested at least 10 times and the data in Fig. 6a represent the average values obtained after 1000 s of measurement. It is therefore evident from this figure that the 2D Au-ZnO heterostructures were almost insensitive to all added chemicals confirming superior selectivity towards the amperometric H2O2 detection at room temperature.
Finally, the long-term stability testing is organized and executed for 30 consecutive days with periodical testing every 6 days. The measured results of this testing exhibited that the sensor’s response during the trial has only decreased ~ 3% after 30 days of continuous measurements. This fact reassured that in addition to the main investigated sensing characteristics, the ALD-fabricated nanoscale Au-ZnO heterostructure possesses great long-term stability towards H2O2 amperometric measurements.
The enhanced mechanism of the amperometric H2O2 detection for the Au-ZnO heterostructures is presented as the schematic band diagram in Fig. 6b. The improvement in H2O2 detection by the Au-ZnO heterostructures can be explained by the following reasons. First, the Au-ZnO heterostructures possess a unique tortuous nanostructure ensuring high surface-to-volume ratio and abundance of the adsorption centers on the surface and in the bulk of a heterostructure. Secondly, a tortuous Au-ZnO nanostructure provides enhanced specific surface area as well as big pore sizes with diffusion channels to the measuring chemical, so that the inner surface of the heterostructure would also able to have sufficient contact with H2O2. Thirdly, junctions between these small nanoparticles in the heterostructure are indistinguishable to the thin film grain boundaries. Thus, the adsorption of reactive O− oxygen ions enabled by high concentrations of the oxygen vacancies developed in the Au-ZnO heterostructure [73, 74]. Fourth, the improved H2O2 sensitivity is also implemented by the establishment of a well-developed Au-ZnO interface during post-annealing. In regard to electronic sensitization effect, for ZnO, as a typical n-type semiconductor, its work function of 4.65 eV is smaller than the work function of Au (5.1 eV) . Consequently, the electrons tend to transfer from a high energy state (ZnO) to a low energy state (Au). Therefore, as for the Au-ZnO heterostructure, a Schottky contact between Au and ZnO would form at the thermal equilibrium state. Accordingly, the Schottky contacted between Au and ZnO results in the generation of a thick depletion layer at the Au-ZnO interface as presented in Fig. 6b. The depletion layer on the Au-ZnO interface was a thick space charge layer in contrast to the bare ZnO-based sensors, which only had a thin surface depletion layer . This not only causes an increase in the resonant electron density but also creates energetic electrons in the higher energy states. As a result, these resonant electrons are so active that they can transfer back to the conduction band of ZnO upon its exposure to the detecting H2O2 chemical, which affects the reduction of the thickness of the electron depletion layer. Moreover, during oxidation of H2O2, the presence of Au in the Au-ZnO heterostructure reduces the Schottky barrier, which subsequently ensures an easier and faster way for the sensing reaction .
All major characteristics of the various electrochemical, colorimetric, fluorometric, and chemiluminescent H2O2 detectors are summarized in Table 2. The results obtained for ALD-fabricated Au-ZnO heterostructures can clearly confirm that the 2D Au-ZnO heterostructures have superior performance compared with the other modified ZnO-based nanostructures. Specifically, results showed that our sensors have the widest linear range and the lowest LOD value compatible with the best LOD values among all reported electrochemical, chemiluminescent, colorimetric, and fluorometric H2O2 detectors. Therefore, Au-ZnO heterostructures are very attractive and reliable candidates for the further development of practical H2O2 measuring devices.
In this study, wafer-scale nanometer-thick 2D ZnO films were successfully fabricated on the nanostructured Au electrodes by the ALD technique using (C2H5)2Zn and H2O precursors, respectively. Then, for the development of Au-ZnO heterostructures, 2D ZnO films were subjected to post-annealing at 250 °C for 3 h. After annealing, the H2O2-sensing capabilities of Au-ZnO heterostructures were subsequently investigated. Intensive testing revealed that Au-ZnO heterostructures showed excellent sensing capabilities towards amperometric H2O2 detection, principally at the low concentration level. 2D Au-ZnO heterostructures displayed a high sensitivity of 0.53 μA μM−1 cm−2, the widest linear H2O2 concentration range of 1.0 μM–120 mM among all reported different H2O2 sensors, very low LOD of 0.78 μM, fast response-recovery time (~ 2.0 s), excellent selectivity in the presence of various interfering chemical agents, and outstanding long-term stability. Additionally, the development of Au-ZnO nano-interface and high surface-to-volume ratio in heterostructures enabled highly expanded specific surface area of heterostructure, allowing the measuring chemical agent to reach inside of the heterostructure more easily. Consequently, the study of 2D Au-ZnO heterostructures indisputably validated the fact that these heterostructures can be considered as one of the valuable candidates for the design of practical electrochemical H2O2 devices.
Availability of Data and Materials
Surface morphology of the samples was investigated by FE-SEM (Fig. 2). The chemical bonding and crystal structure of the ALD-fabricated samples were characterized by FTIR (Fig. 2), XPS (Fig. 3), Raman spectroscopy (Fig. 4), electrochemical impedance spectroscopy (Fig. 4), and CV measurements (Figs. 5 and 6).
Atomic force microscopy
Atomic layer deposition
Chemical vapor deposition
Energy dispersive spectroscopy
Field emission scanning electron microscopy
Fourier Transform Infrared
Electrochemical impedance spectroscopy
Scanning electron microscopy
X-ray photoelectron spectroscopy
Akbari MK, Zhuiykov S (2019) A bioinspired optogenetically engineered artificial neurorobotics device with sensorimotor functionalities. Nat Communic. 10:3873
Zhuiykov S, Kats E (2013) Atomically-thin two-dimensional materials for functional electrodes of electrochemical devices: A review. Ionics 19:825–865
Xu H, Han F, Xia C et al (2019) Wafer-scale fabrication of sub-10 nm TiO2-Ga2O3 n-p heterojunctions with efficient photocatalytic activity by atomic layer deposition. Nanos Res Lett. 14:163–173
Hai Z, Zhuiykov S (2018) Functionalizing new intercalation chemistry for sub-nanometer-scaled inter-layer engineering of 2D transition metal oxides and chalcogenides. Adv Mat Interf. 5:1701385
Osada M, Sasaki T (2012) Two-dimensional dielectric nanosheets: novel nanoelectronics from nanocrystal building blocks. Adv Mater. 24:210–228
Zappa D, Galstyan V, Kaur N et al (2018) Metal oxide -based heterostructures for gas sensors - a review. Anal Chim Acta 1039:1–23
Ramachandran RK, Dendooven J, Filez M et al (2016) Atomic layer deposition route to tailor nanoalloys of noble and non-noble metals. ACS Nano 10:8770–8777
Zhuiykov S, Hyde L, Hai Z et al (2017) Atomic layer deposition-enabled single layer of tungsten trioxide across a large area. Appl Mater Today 6:44–53
Wei Z, Hai Z, Akbari MK et al (2018) Ultrasensitive, sustainable, and selective electrochemical hydrazine detection by ALD-developed two-dimensional WO3. Chem Electro Chem 5:266–272
Zhuiykov S (2016) Material characterisation and transistor function of quasi two-dimensional substoichiometric WO3-x nanoflakes. Mater Lett. 173:173–177
Zhuiykov S, Kats E, Carey B, Balendhran S (2014) Proton intercalated two-dimensional WO3 with enhanced charge-carrier mobility at room temperature. Nanoscale 6:15029–15036
Zhuiykov S, Akbari MK, Hai Z et al (2017) Wafer-scale fabrication of conformal monolayer TiO2 by atomic layer deposition using tetrakis (dimethylamino) titanium and H2O precursors. Mat Design 120:99–108
Xie Q, Jiang YL, Detavernier C et al (2007) Atomic layer deposition of TiO2 from tetrakis-dimethyl-amido titanium or Ti isopropoxide precursors and H2O. J Appl Phys. 102:083521
Wei Z, Hai Z, Akbari MK et al (2018) Atomic layer deposition-developed two-dimensional α-MoO3 windows excellent hydrogen peroxide electrochemical sensing capabilities. Sens Actuators B 262:334–344
Xu H, Arbari MK, Hai Z et al (2018) Two-dimensional MoO3 goes wafer-scaled nano-architectonics by atomic layer deposition. Mat Design 149:135–144
Akbari MK, Hai Z, Depuydt S et al (2017) Highly-sensitive, fast-responding and stable photodetector based on ALD-developed monolayer TiO2, IEEE Trans. Nanotechn. 16:880–887
Akbari MK, Hai Z, Wei Z et al (2018) ALD-developed plasmonic two-dimensional Au-MoO3-TiO2 heterojunction architectonics for design of photovoltaic devices. ACS Appl Mat Interf. 10:10304–10314
Wei Z, Akbari MK, Hai Z et al (2019) Ultra-thin sub-10 nm Ga2O3-WO3 heterostructures developed by atomic layer deposition for sensitive and selective C2H5OH detection on ppm level. Sens Actuators B 287:147–156
Akbari MK, Hai Z, Wei Z et al (2019) Naturally occurring surface oxide of liquid metal galinstan and its p-n heterojunctions for optoelectronic applications. J Mater Chem C 7:5584–5595
Hai Z, Akbari MK, Xue C et al (2017) Photodetector with superior functional capabilities based on monolayer WO3 developed by atomic layer deposition. Sens Actuators B 245:954–962
Wang Y, Wan Y, Zhang DY et al (2016) Zhang, Reduced graphene sheets modified glassy carbon electrode for electrocatalytic oxidation of hydrazine in alkaline media. Electrochem Comm. 12:187–190
Teodoro KBR, Migliorini FL, Christinelli WA, Correa DS (2019) Detection of hydrogen peroxide (H2O2) using a colorimetric sensor based on cellulose nanowhiskers and silver nanoparticles. Carbohyd Pol. 212:235–241
Liu M, Yu YX, Zhang WD (2017) A non-enzymatic hydrogen peroxide photoelectrochemical sensor based on a BiVO4 electrode. Electroanalysis 29:305–311
Chang Q, Deng K, Zhu L (2009) Determination of hydrogen peroxide with the aid of peroxidase-like Fe3O4 magnetic nanoparticles as the catalyst. Microchim Ichnoanal Acta 165:299
Lu Y, Ye W, Yang Q (2016) Three-dimensional hierarchical porous PtCu dendrites: a highly efficient peroxidase nanozyme for colorimetric detection of H2O2. Sens. Actuators B 230:721–730
Cichosz S, Masek A, Zaborski MS (2018) Polymer-based sensors: a review. Pol Testing 67:342–348
Gholami M, Koivisto BM (2019) A flexible and highly selective non-enzymatic H2O2 sensor based on silver nanoparticles embedded into Nafion. Appl Surf Sci. 467–468:112–118
Khan SB, Rahman MM, Asiri AM et al (2014) Fabrication of non-enzymatic sensor using Co doped ZnO nanoparticales as a marker of H2O2. Physica E 62:21–27
Ke X, Zhu G, Dai Y, Shen Y, Liu J (2018) Fabrication of Pt-ZnO composite nanotube modified electrodes for the detection of H2O2. J Electroanal Chem. 817:176–183
Rui Q, Komori K, Tian Y, Liu H, Luo Y, Sakai Y (2010) Electrochemical biosensor for the detection of H2O2 from living cancer cells based on ZnO nanosheets. Anal Chim Acta 670:57–62
Xue B, Li K, Gu S, Zhang L, Lu J (2018) Ni foam-supported ZnO nanowires and Co3O4/NiCo2O4 double-shelled nanocages for efficient hydrogen peroxide detection. Sens Actuators B 262:828–836
Chen L, Xu X, Cui F, Qiu Q, Xu J (2018) Au nanoparticles-ZnO composite nanotubes using natural silk fibroin fiber as template for electrochemical non-enzymatic sensing of hydrogen peroxide. Anal Biochem. 55:1–8
Hussain M, Sun H, Karim S, Nisar A, Khan M, Haq AU, Iqbal M, Ahmad M (2016) Noble metal nanoparticle-functionalized ZnO nanoflowers for photocatalytic degradation of RhB dye and electrochemical sensing of hydrogen peroxide. J Nanopart Res. 18:1–14
Wang Q, Zheng J (2010) Electrodeposition of silver nanoparticles on a zinc oxide film: improvement of amperometric sensing sensitivity and stability for hydrogen peroxide determination. Microchim Acta 169:361–365
Pinter JS, Brown KL, DeYoung PA, Peaslee GF (2007) Amperometric detection of hydrazine by cyclic voltammetry and flow injection analysis using ruthenium modified glassy carbon electrodes. Talanta 71:1219–1225
Yang X, Guo Y, Mei Z (2009) Chemiluminescent determination of H2O2 using 4-(1,2,4-triazol-1-yl) phenol as an enhancer based on the immobilization of horseradish peroxidase onto magnetic beads. Anal Biochem. 393:56–61
Hanaoka S, Lin JM, Yamada M (2001) Chemiluminescent flow sensor for H2O2 based on the decomposition of H2O2 catalyzed by cobalt(II)-ethanolamine complex immobilized on resin. Anal Chim Acta 426:57–64
Kysil DV, Vasin AV, Sevostianov SV et al (2017) Formation and luminescent properties of Al2O3:SiOC nanocomposites on the base of alumina nanoparticles modified by phenyltrimethoxysilane. Nanoscale Res Lett. 12:477
Liu T, Zhang S, Liu W et al (2020) Smartphone based platform for ratiometric fluorometric and colorimetric determination H2O2 and glucose. Sens Actuators B 305:127524
Liu W, Ding F, Wang Y (2018) Fluorometric and colorimetric sensor array for discrimination of glucose using enzymatic-triggered dual-signal system consisting of Au@Ag nanoparticles and carbon nanodots. Sens Actuators B 218:310–317
Li SJ, Zhang JC, Li J et al (2018) 3D sandwich structured hybrid of gold nanoparticles decorated MnO2/graphene-carbon nanotubes as high performance H2O2 sensors. Sens Actuators, B 260:1–11
Ahmad R, Beduk T, Manohar Majhi S, Nabil Salama KR (2019) One-step synthesis and decoration of nickel oxide nanosheets with gold nanoparticles by reduction method for hydrazine sensing application. Sens Actuators B 256:139–147
Wei Z, Hai Z, Karbalaei Akbari M et al (2019) Surface functionalization of wafer-scale two-dimensional WO3 nanofilms by NM electrodeposition (NM=Ag, Pt, Pd) for electrochemical H2O2 reduction improvement. Electrochem Acta 297:417–428
Yin Y, Alivisatos AP (2004) Colloidal nanocrystal synthesis and the organic-inorganic interface. Nature 437:664
Lin CY, Lai YH, Balamurugan A et al (2010) Electrode modified with a composite film of ZnO nanorods and Ag nanoparticles as a sensor for hydrogen peroxide. Talanta 82:340–347
Boyadjiev SI, Georgieva V, Yordanov R et al (2016) Preparation and characterization of ALD deposited ZnO thin films studied for gas sensors. Appl Surf Scie. 387:1230–1235
Sahoo T, Nayak SK, Chelliah P et al (2016) Observations of two-dimensional monolayer zinc oxide. Mat Res Bull. 75:1340138
Sun Y, Wei Z, Zhang W et al (2016) Synthesis of brush-like ZnO nanowires and their enhanced gas-sensing properties. J Mater Sci. 51:1428–1436
Wang C, Ma S, Sun A et al (2014) Characterization of electrospun Pr-doped ZnO nanostructure for acetic acid sensor. Sens Actuators B 193:326–333
Yoo R, Guntner AT, Park Y et al (2019) Sensing of acetone by Al-doped ZnO. Sens Actuators B 283:107–115
Tang YL, Li ZJ, Ma JY et al (2014) Ammonia gas sensors based on ZnO/SiO2 bi-layer nanofilms on ST-cut quartz surface acoustic wave devices. Sens Actuators B 201:114–121
Partharathy S, Nandhini V, Jeyaprakash BG (2016) Improved sensing response of photo activated ZnO thin film for hydrogen peroxide detection. J Coll Interf Scie. 482:81–88
Wang T, Kou X, Zhao L et al (2017) Flower-like ZnO hollow microspheres loaded with CdO nanoparticles as high performance sensing material for gas sensors. Sens Actuators B 250:692–702
Shu-Wen X (2012) A Study of annealing time effects on the properties of Al:ZnO. Phys Procedia 25:345–349
Al-Asedy HJ, Bidin N, Abbas KN, Al-Azawi MA (2016) Structure, morphology and photoluminescence attributes of Al/Ga co-doped ZnO nanofilms: Role of annealing time. Mat Res Bull. 97:71–80
Srivastava AK, Praveen M, Arora SK et al (2010) Nanostructural features and optical performance of RF magnetron sputtered ZnO thin films. J Mater Sci Techn 26:986–990
Patil SS, Mali MG, Tamboli MS et al (2016) Green approach for hierarchical nanostructured Ag–ZnO and their photocatalytic performance under sunlight. Catal Today 260:126–134
Das D, Mondal PD (2014) Photoluminescence phenomena prevailing in c-axis oriented intrinsic ZnO thin films prepared by RF magnetron sputtering. RSC Adv. 4:35735
Casaletto MP, Longo A, Martorana A et al (2006) XPS study of supported gold catalysts: the role of Au0 and Au+δ species as active sites. Surf Interf Anal. 38:215–218
Ohta T, Shibuta M, Tsunoyama H et al (2013) Size and structure dependence of electronic states in thiolate-protected gold nanoclusters of Au25(SR)18, Au38(SR)24, and Au144(SR)60. J Phys Chem C 117:3674–3679
Fong YY, Visser BR, Gascooke JR et al (2011) Photoreduction kinetics of sodium tetrachloroaurate under synchrotron soft X-ray exposure. Langmuir 27:8099–8104
Anderson DP, Alvino JF, Gentleman A et al (2013) Chemically-synthesised, atomically-precise gold clusters deposited and activated on titania. Phys Chem Chem Phys. 15:3917–3929
Mazzaglia A, Scolaro LM, Mezzi A et al (2009) Supramolecular colloidal systems of gold nanoparticles/amphiphilic cyclodextrin: a FE-SEM and XPS investigation of nanostructures assembled onto solid surface. J Phys Chem C 113:12772–12777
Ganesh RS, Navaneethan M, Mani GK et al (2017) Influence of Al doping on the structural, morphological, optical, and gas sensing properties of ZnO nanorods. J Alloys Compd. 698:555–564
Wang J, Li Y, Kong Y et al (2015) Non-fluorinated superhydrophobic and micro/nano hierarchical Al doped ZnO film: the effect of Al doping on morphological and hydrophobic properties. RSC Adv. 5:81024–81029
Choi KI, Hwang SJ, Dai Z et al (2014) Rh-catalyzed WO3 with anomalous humidity dependence of gas sensing characteristics. RSC Adv. 4:53130–53136
Paraguay DF, Miki-Yoshida M, Morales J et al (2000) Influence of Al, In, Cu, Fe and Sn dopants on the response of thin film ZnO gas sensor to ethanol vapour. Thin Solid Films 373:137–140
Sundara Venkatesh P, Ramakrishnan V, Jeganathan K (2016) Raman silent modes in vertically aligned undoped ZnO nanorods. Physica B 481:204–208
Bundesmann C, Ashkenov N, Schubert M et al (2003) Raman scattering in ZnO thin films doped with Fe, Sb, Al, Ga, and Li. Appl Phys Lett. 83:1974
Kaschner A, Haboeck U, Strassburg M et al (2002) Nitrogen-related local vibrational modes in ZnO:N. Appl Phys Lett. 80:1909
Ahmad R, Tripathy N, Ahn MS et al (2017) Highly efficient non-enzymatic glucose sensor based on CuO modified vertically-grown ZnO nanorods on electrode. Scien Rep. 7:5715
Shen CL, Lou Q, Lv CF et al (2019) Bright and multicolor chemiluminescent carbon nanodots for advanced information encryption. Adv. Sci. 6:1802331
Zhang Y, Xu JQ, Xiang Q et al (2009) Brush-like hierarchical ZnO nanostructures: synthesis, photoluminescence and gas sensor properties. J Phys Chem C 113:3430–3435
Shipway AN, Lahav M, Gabai R, Willner I (2000) Investigations into the electrostatically induced aggregation of Au nanoparticles. Langmuir 16:8789–8795
Pan YN, Wu GD, He YF, Feng JT, Li DQ (2019) Identification of the Au/ZnO interface as the specific active site for the selective oxidation of the secondary alcohol group in glycerol. J Catal 369:222–232
Jia W, Guo M, Zheng Z et al (2009) Electrocatalytic oxidation and reduction of H2O2 on vertically aligned Co3O4 nanowalls electrode: Toward H2O2 detection. J Electroanal Chem. 625:27–32
Liu D, Wan J, Wang H et al (2019) Mesoporous Au@ZnO flower-like nanostructure for enhanced formaldehyde sensing performance. Inorg Chem. Comm. 102:203–209
S.Z. acknowledges the support from the “100 Talents Program” of Shanxi province, People’s Republic China. The work was performed in part at the Melbourne Center for Nanofabrication (MCN) in the Victoria Node of the Australian National Fabrication Facility (ANFF). Z.W. is thankful for the aid from Gent University, Belgium, for her BOF Grant (BOF17/STA/015).
This study was supported and funded by the Gent University BOF Grant (BOF17/STA/015).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Ellipsometry data for deposition of thicker ZnO for building reliable optical constants (a), device schematic indicating Au/Cr pads in dark green (separated by 200 μm) and the dicing/alignment in markers in light green (20 μm) (b), microcrograph of the edge of four individual devices, as per the mask design a 40 μm gap is allotted for dicing and each Au/Cr pad is inset from the edge of the 1.0 x 1.0 cm die by 50 μm (c), micrograph of 200 m Au/Cr pad separation of 2 individual devices (d) with 3D AFM image of Au/Cr layer step height (e). Figure S2. Experimental and model generated data for variable angle spectroscopic ellipsometric measurements of ALD developed ZnO with initial thickness of (a) 0.9 nm and (b) 1.3 nm.
About this article
Cite this article
Xu, H., Wei, Z., Verpoort, F. et al. Nanoscale Au-ZnO Heterostructure Developed by Atomic Layer Deposition Towards Amperometric H2O2 Detection. Nanoscale Res Lett 15, 41 (2020). https://doi.org/10.1186/s11671-020-3273-7
- Atomic layer deposition
- Amperometric detection